DURABILITY OF MORTAR LININGS IN DUCTILE IRON PIPES
DURABILITY OF MORTAR LININGS IN DUCTILE IRON PIPES
Durability of mortar linings
I. S. MELAND
SINTEF Civil and Environmental Engineering, Cement and Concrete, Trondheim,
Durability of Building Materials and Components 8. (1999) Edited by M.A. Lacasse
and D.J. Vanier. Institute for Research in Construction, Ottawa ON, K1A 0R6,
Canada, pp. 170-179.
National Research Council Canada 1999
Mortar linings in ductile iron pipes for distribution of water have been investigated
with respect to micro-structure, composition, durability and leach of chemical
components. Scanning Electron Microscopy (SEM) and Wave Dispersive Analysis
of X-ray (WDAX) have been used to study degradation of mortar linings which have
been in service for 10 - 20 years. The same techniques have also been used to follow
degradations and leaching of new mortar linings exposed to aggressive solutions in
laboratory. Relatively good correlation has been found between the laboratory tests
and the degradation of linings of pipes in service. Reliable methods for examination
and testing of mortar linings in new pipes will definitely be a valuable implement for
municipal water works to specify a wanted composition and quality of mortar linings.
Keywords: water pipes, mortar linings, type of cement, durability
Among our building materials few of them affect our daily life as much as the
water pipe line network. A steady delivery of water without any interruptions is of
great importance to our quality of life. Also from an economic point of view it is
important to have pipes of good quality in order to secure a long service life of the
pipes without considerable expenses of maintenance. Traditionally, water mains
consisted of ductile iron pipes without any protection against corrosion. From about
1970 - 80 internally mortar lined iron pipes came into use in Norway. Due to a high
pH the mortar linings are supposed to protect the iron pipes against corrosion.
However, dependent on physical and chemical properties of the mortar and / or the
quality of the water, any mortar lining is to be more or less attacked by the streaming
water, and chemical compounds like calcium and alkalies are leached from the mortar
linings. Unfortunately, the greater part of the water supply in our country comes from
surface water. Drinking water has a low pH (average: 6.7), a low hardness (average:
Ca2+ = 2.6 mg/l), and a low alkalinity (average: 0.05 - 0.1 mmol/l). Most of the local
water works are small and cannot afford to invest in water treatment equipment to
increase pH and mineral content by adding lime or alkalies. Often the results are a
comparatively short "service life" of mortar linings, which means great expences on
maintenance, repairs, and replacements of pipes, and bad water-quality due to leach
of chemical components from the mortar.
The capacity of mortar and concrete to withstand chemical degradation can be
related to three of the material's characteristica:
deeper into the mortar lining, the mortar may lose its capacity to protect the iron pipe
Methods of lining
Commonly two methods are used for lining of ductile iron pipes:
Centrifugal method. The mortar mix is cast on the iron pipe when it is under a
very high rotation velocity. This gives a cement mortar lining with a very cement
rich layer towards the water with a porous and sand rich layer towards the iron
pipe. A scanning microscope photo of the micro structure of this lining is shown
in Figure 1.
Fig. 1: Centrifugal lining method
Centrifugal projection head method. By this method the mortar mix is cast on a
still-lying iron pipe through a spinning head. This gives a cement mortar lining
with an equal distribution of cement paste, pores and sand throughout the whole
thickness of the lining. A scanning microscope photo of the micro structure of
this lining is shown in Figure 2.
Fig. 2: Centrifugal projection head method
If the mortar lining is exposed to soft water with low pH and low content of
minerals, the type of cement used in the mortar may have decisive consequences for
the durability of the lining. According to DIN 2614 following cements are allowed
for mortar linings in pipes transporting drinking water, Ordinary Portland Cement
(OPC), High Alumina Cement (HA cement), Blast Furnace Slag Cement (BFS
cement), Fly Ash Cement (FA cement), and Sulphate Resistant Portland Cement (SR
cement). One of the main components of a hardened OPC paste is calcium hydroxide
[Ca(OH)2], and this is also the "weak" mineral of a cement paste and is easily
leached from a cement mortar. Among the cements mentioned, OPC and SR cement
have the larger contents of calcium hydroxide. Due to the raw materials HA cement
is relatively low in Ca(OH)2. Also mortars based on BFS cement and FA cement
have reduced content of Ca(OH)2 partly due to the lower content of OPC in these
cements and partly because of the pozzolan reaction between calcium hydroxide and
the mineral substitute in the cements.
The aim of the project was to find which of the mortar linings is the most
suitable one for a specific water quality. This should be done by, firstly, to carry out a
condition survey of mortar linings taken from existing pipes lines at different parts of
the country. Secondly, to use accelerated laboratory test methods to investigate the
durability of specimens taken from new linings, and to examine the conformity
between the laboratory tests and the actual deterioration caused in performance by
The experiments included mortar linings based on either Ordinary Portland
Cement, High Alumina Cement, Blast Furnace Slag Cement, or Fly Ash Cement.
5.2.1 Scanning electron microscope (SEM)
The mortar linings have been investigated by use of Scanning Electron
Microscope (SEM). Using Back Scattered Electron modus (BSE) in Scanning
Electron Microscope (SEM) for examination of mortar gives the possibility to
distinguish between different phases and their distribution. It is important that the
sample is properly plane polished. The back scatter process depends strongly on the
average atom number of the sample, sample density and the energy of the primary
electrons. Phases with high average atom number, as iron (Fe), and / or samples with
a dense structure will have bright colours on a BSE image. On the other hand, phases
with low average atom number, as magnesium, and samples with porous structures
will appear dark.
5.2.2 Wave dispersive analysis of X-rays (WDAX).
Together with a SEM-investigation Wave Dispersive Analysis of X-rays
(WDAX) diagrams have been recorded. WDAX gives semiquantitative compositions
of solids. The principle for the method is based upon the exitement of the electrons
of each atom in the sample. When the electrons return to their stable energy level, the
atoms in the sample will emit X-rays of a certain energy specific for each chemical
element. The results will appear as peaks in a diagram with variation of energy as Xaxis. The position (X) determines the element, while the height (Y) of the peaks
gives the amount of the spesific elements in the sample. By use of WDAX small
volumes (≈ 1 µm3) of a sample are analysed with respect to chemical composition.
5.2.3 Accelerated Leaching Test
An accelerated leaching test has been performed by using a modification of the
Dutch method NEN 7345. According to this method samples of concrete or mortar
are exposed to deionized water or acid solution for 64 days. At certain intervals
during this period samples are taken from the solutions and analysed with respect to
calcium and aluminium.
5.3.1 Mortar linings in used pipes
Specimens of mortar linings were impregnated with epoxy and plane polished.
Deterioration of the mortars has been studied by use of scanning electron microscope
(SEM) and wave dispersive analysis of x-rays (WDAX). In addition leaching of
elements (CaO and Al2O3) from the matrix has been determined by analysing the
cement pastes at certain distances from the water side towards the side of the iron
5.3.2 Mortar linings in new pipes
For accelerated deterioration tests of mortar linings specimens of about 130 x 70
mm were cut from the pipes, isolated by epoxy, and exposed to acetic acid buffer
solution (pH = 4,6) for 64 days. The solution was kept in movement throughout the
testing period. A buffer solution was chosen for the experiments because the buffer
solution gives a relatively permanent pH even when Ca(OH)2 is leached from the
mortar. This gives allowance to compare a buffer solution with streaming water.
During the exposure period samples have been taken from the solutions and analysed
with respect to contents of calcium (Ca2+) and aluminium (Al3+) by use of atomic
absorption spectrophotometer. Durability of the mortar linings has been estimated by
SEM / WDAX examinations of the specimens before and after exposure. In addition
the thickness of the linings has been measured before and after exposure in the buffer
Results and discussion
Mortar linings from pipes taken from networks
The investigation included 15 mortar lined iron pipes taken from pipelines at
several water works throughout the country. The pipes had been in use for 10 - 20
years. SEM (BSE) and WDAX showed following results:
The cements used in the mortars were Ordinary Portland, Blast Furnace Slag
Cement or Fly Ash Cement.
• Both the centrifugal method and the centrifugal projection head method had been
used in lining the pipes.
All the specimens showed degradation of the mortar lining in form of leached
elements. This means that water delivered to the people (consumers) may not have
the wanted quality due to a high pH caused by leaching of calcium and hydroxyl ions
from the mortars. At the same time the leaching of calcium hydroxide also causes a
gradually loss of capacity to protect the iron pipe against corrosion. A typical SEM
photo of a mortar lining taken from a network is shown in Figure 3. Three distinct
layers can be seen on the photo. That means a gradually leaching of the cement paste.
The black area at the bottom of the photo, which shows the "water side" of the
mortar, indicates a strongly leached paste, whilst the inner white area indicates that no
leaching of elements has occurred.
Fig. 3: Leached mortar linings
A considerable reduction of the linings' thickness could be observed in some of
the pipes, especially in those lined by the centrifugal projection head method.
Linings from a couple of pipes which had been exposed for about 20 years to
water quality: pH = 6.5, calcium (Ca2+) = 1,5 mg / l, alkalinity = 0.04 mmol / l, were
totally destroyed, and by SEM / WDAX iron rich layers could be observed in the
remaining mortar lining. This result indicates that corrosion of the iron pipes has
Due to these results, which showed that mortar linings could be in a rather bad
condition after 10 - 20 years in use, it was decided to do some laboratory tests on new
mortar linings in order to evaluate which type of mortar i. e. cement and method of
lining were the most durable one.
Mortar linings in new pipes
The investigation included mortar linings based on the following types of
cement, FA cement, BFS cement, and HA cement. The mortar based on FA cement
had been cast on to the iron pipe by the centrifugal projection head method. Whilst
the centrifugal method had been used in lining the pipes with the BFS cement and HA
Measurements of the linings' thickness before and after exposure in acetic acid
buffer solution showed:
• Non reduction in thickness of the mortar based on HA cement.
• A reduction of 0.5 - 1.0 mm of the mortar based on BFS cement.
• A reduction of about 3 mm of the mortar based on FA cement.
6.2.1 Accelerated leaching test
The total quantities of calcium and aluminium leached from the mortars during
64 days are given in table 1. The results are calculated as oxides, and given in mg /
cm2 exposed mortar surface.
Table 1: Leached CaO and Al2O3 (mg / cm2) from mortar linings after 64 days of
exposure in acetic acid buffer solution.
CaO (mg/cm )
Type of cement
The relatively large quantity of Al2O3 leached from the HA cement based
mortar, is due to the raw material used in the production of this cement. When
following the quantities of leached Ca and Al from the mortars at each testing time,
the results indicated a very rapid leaching from the mortars based on FA cement and
BFS cement, respectively. The leaching from the HA cement based mortar, however,
went on through a longer period of time.
6.2.2 SEM / WDAX
SEM / WDAX examinations showed leached linings into a depth of 0.75 mm
for the HA cement based mortar. Corresponding results were 1.5 mm and 2.0 mm
respectively for the FA cement and the BFS cement based mortars. It should be
noticed, however, the great reduction of thickness of the FA cement based lining
during the test period. A WDAX diagram with respect to leached Ca and Al from the
HA cement mortar is shown on Figure 4.
Fig. 4: High Alumina mortar. Content of CaO andAl2O3 before- and after
The results from the accelerated test indicated following:
When exposed to concrete aggressive solution, mortars cast on to the iron pipe by
the centrifugal projection head method seems to lose material to a larger degree
than mortars cast on to the iron pipe by the centrifugal method. This has also
been observed in examinations of used pipes taken from networks. This means
that the dense cement layer obtained by the centrifugal method, has avery small
Mortar based on High Alumina cement is more durable in concrete aggressive
solutions with low pH compared to the other mortars included in the experiment.
This means that a High Alumina cement based mortar lining will have a longer
“service life” at low pH than linings based on Blast Furnace Slag cement or Fly
The smallest total amounts of calcium and aluminium leached into the solution
were measured from the Blast Furnace Slag cement.
Rather unexpected high amounts of calcium and aluminium were leached from
High Alumina cement mortar.
Based on the results from the accelerated test programme, ductile iron pipes
lined by the centrifugal method with mortar based on Blast Furnace Slag cement, can
be recommended for pipelines, which are going to be exposed to a moderate water
For extreme water qualities, water with low pH, low content of calcium and low
alkalinity, High-Alumina cement based mortar linings should be recommended.
Østerhus, S. SINTEF Civil and Environmental Engineering, Trondheim, Norway.
DIN 2614 "Zementmörtelauskleidungen für Gussröhre, Stahlröhre und Formstücke;
Verfahren, Anforderungen, Prüfungen".
NEN 7345 "Leaching Characteristics of Building and Solid Waste Materials.
Leaching Tests. Determination of the leaching Behaviour of Inorganic
Components from shaped Building Materials, Monolithic and Stabilized